- Research article
- Open Access
Two-month longitudinal study of mechanical properties of absorbable sutures used in orthopedic surgery
Journal of Orthopaedic Surgery and Research volume 11, Article number: 111 (2016)
This is the first study assessing the properties of large-diameter degradable sutures relevant for orthopedic applications over the course of in vitro incubation for 2 months. The data we present here provide guidance to the orthopedic surgeon in predicting the long-term performance of suture materials used everyday in surgical practice.
Five different absorbable (Vicryl, Maxon, Monocryl, PDS II, Vicryl rapide) and one non-absorbable (Ethibond) suture materials were tested. Measurements were made at five time points during the 56 days of incubation under physiological conditions (37.0 ± 0.02 °C; pH 7.4 ± 0.2). The following variables were recorded: load to failure, strain at maximal load as elongation normalized to original length, stiffness as the ratio of load to displacement on the linear proportion of the stress strain curve, and hysteresis as area under the curve of the stress strain curve.
Vicryl was the strongest fiber on day 0 (195 N); however, by day 42, the tensile strength of the suture reduced to 14 N. Between days 14 and 28, PDS II (171 N) and Maxon (182 N) sustained the highest loads. Monocryl (p = 0.003) and Maxon (p < 0.001) showed an increasing strain with time, whereas Vicryl (p = 0.002) and Vicryl rapide (p = 0.007) revealed an increasing material stiffness. Furthermore, both Vicryl (p = 0.053) and Monocryl (p < 0.001) had an increasing hysteresis with ongoing degradation. Maxon, PDS II, and Ethibond showed stable material properties during the 2 months.
The three absorbable sutures Vicryl, PDS II, and Maxon could sustain higher loads during the first 2 weeks than the non-absorbable Ethibond. Unexpectedly, Maxon and PDS II maintained their elastic properties in spite of their proceeding degradation and loss of tensile strength.
Medical suture material is essential to appropriately position and hold tissue until healing has occurred. Particularly in orthopedic surgery, the suture material may be subjected to considerable mechanical loads for a long time period, as healing after tendon, ligament, or fascia repair takes place over two or more postoperative months.
Because the suture is often no longer needed after healing, different biodegradable suture materials have been developed and are in widespread surgical use. The materials used in such sutures can differ not only in tensile properties like strength and stiffness but also in knot strength. Data on longitudinal retention of mechanical strength is usually available over a limited time frame from the suture manufacturer. Yet, a thorough description of the suture’s mechanical behavior (e.g., stiffness, hysteresis) over a time frame relevant to musculoskeletal injuries has not been reported, despite the fact that substantial changes of these properties with suture degradation is certain [1, 2].
The speed of suture degradation caused by hydrolysis depends not only on the material but also on the fiber diameter, tissue temperature, and pH [3–5]. Biodegradation of absorbable sutures has been studied in the discipline of visceral surgery, whereas such fibers are too weak for orthopedic purposes [6–10]. There is no data available regarding time-dependent mechanical properties of absorbable sutures for large-diameter fibers including sizes United States Pharmacopeia (USP) 0 and more. The existing data remains limited regarding the influence of time or focuses on highly specific orthopedic applications involving arthroscopic surgery and bone anchors [11–16].
Therefore, we set out to characterize how (1) failure load, (2) failure strain, (3) suture stiffness, and (4) suture hysteresis of six different suture materials would vary over the course of in vitro incubation for 2 months. We hypothesized that longitudinal changes in suture mechanical properties would be highly material dependent and possibly more important the pure development of failure load as stated by the manufacturers.
We tested five different absorbable and one non-absorbable suture materials that are used daily in orthopedic surgery (see Table 1). All the sutures were chosen with a diameter of USP 1, being an appropriate size for suture of fascia, capsule, and tendons. Furthermore, it is the largest diameter in every tested suture material that is available. In preparation for testing, the needle was removed and the sutures were circled around a metallic cylinder with a diameter of 12 cm (see Fig. 1a). Each suture loop was tied with five standard surgical square knots. A single surgeon tied all the knots. From each suture type, 60 loops were produced in the described matter.
Incubation and fluid
Measurements were made at five time points corresponding to 0, 14, 28, 42, and 56 days of incubation under physiological conditions. All suture materials were incubated together in a polyethylene tube containing 50 ml of a standard testing solution for absorbable materials (see Fig. 1b) . The used solution is approved by ASTM (American Society for Testing and Materials) for testing absorbable sutures. The solution components correspond to ringer solution. As this solution is standardized, it provides reliable comparison of testing results to other mechanical studies of absorbable sutures. All tubes were then kept at a constant temperature of 37.0 ± 0.02 °C. The pH of the solution was buffered to 7.4 ± 0.2 for the whole time of incubation, and the value was controlled before each testing time point.
Measurements on 12 loops were made for each material and at each time point. Samples from each suture material were taken out of the incubator at the appropriate time. Samples were divided into two groups of six loops each of the same material. The loops were fixed in a material testing machine (Zwick1456, Zwick GmbH, Ulm, Germany) as shown in Fig. 1c. The loops were mounted over two metal bars which are moved apart by the machine creating a stress to the fiber.
Using the first group of sutures, load to failure was recorded. For this purpose, loops were pre-tensioned to 1 N and loaded until failure at a rate of 10 mm/s. The second group was used to evaluate the material properties under a repetitive load. After positioning in the testing machine, the loops were pre-tensioned to 1 N. Thirty cycles of load ranging from 1 N to 50 % of the mean load to failure (as measured in the first group) was applied. The loop was then ramp loaded until failure at 10 mm/s. All force displacement data were digitally recorded using the test machine software.
As suture loops (suture/knot construct) were tested in this experiment, the obtained results reflect properties of both suture material and knot security. For this reason, we marked the fiber on each side of the knot to control for knot tightening during the tests. The elongation distance through knot tightening was in all loops insignificant compared to the material elongation.
Analyzing data and statistics
The following variables were recorded for each suture sample: (1) load to failure with and without cyclical loading, (2) elongation of the fiber at maximum load, normalized as the ratio of the end length to the initial loop length, (3) stiffness as the slope of the force/displacement curve in a linear region of the material curve, and (4) hysteresis as the non-elastic energy loss during a cycle of loading and unloading, here normalized as a percentage.
Commercial statistical software (Stata v12.1, StataCorp.) was used for all analyses. Recorded values are indicated as mean with their standard error (mean ± standard error). Graphical results indicate 95 % confidence intervals. A one-way ANOVA was used first to identify differences among the different suture materials, with post hoc analysis of group means using unpaired Student’s t test. The level of significance was set at 0.05.
Load to failure
On day 0, before any incubation, the Vicryl suture showed the highest load to failure (195 ± 4 N). PDS (145 ± 3 N) and Ethibond (145.7 ± 2 N) were on a similar level with no significant difference. Interestingly, the two absorbable fibers Vicryl (195 ± 4 N; p < 0.001) and Maxon (164 ± 7 N; p = 0.036) were both stronger than the non-absorbable Ethibond. The lowest load was detected on Vicryl rapide (51.0 ± 0.9 N).
The development of the load to failure during the 2 months of incubation was characterized (Fig. 2). Even on day 14, the absorbable sutures Vicryl (157 ± 9 N; p = 0.049) and Maxon (183 ± 6 N; p = 0.001) sustained higher loads than the non-absorbable Ethibond (135 ± 1 N), with the Vicryl loops showing the fastest loss of load bearing capacity. After day 42, a conclusive evaluation of Vicryl loops was impossible as the loop was too weak for support the 1-N pre-load. PDS (151 ± 3 N) and Maxon (137 ± 6 N) featured comparable rates of mechanical degradation through day 28, after which the strength of Maxon loops decreased more rapidly (p < 0.001). As expected, the non-absorbable Ethibond loops showed no significant differences over time and had the highest load bearing capacity at the final measurement point (140 ± 2 N). The Monocryl suture was no longer able to sustain the preload of 1 N at day 28, while Vicryl rapide was unable to support load already at day 14.
After applying the cyclic load, the suture loops were again loaded until they failed. In general, there was no significant difference between the load to failure with or without cyclic loading. Exceptions were PDS on day 0 (145 vs. 121 N; p < 0.001) and Maxon at day 14 (183 vs. 155 N; p = 0.044). Ethibond showed a significant difference in ultimate load after cyclical loading at three time points, namely day 0 (146 vs. 134 N; p = 0.04), day 42 (141 vs. 131 N; p = 0.028), and day 56 (140 vs. 126 N; p = 0.028).
Strain at maximal load
The maximal strain of the loop at maximal load on day 0 was highest in Vicryl rapide (57 ± 1.6 %). In PDS and Ethibond, the course was stable. Monocryl (from 13.1 to 30.0 %; p = 0.003) and Maxon (from 14.2 to 35.2 %; p < 0.001) showed an increasing maximal strain with ongoing time (see Fig. 3).
Both Vicryl (from 3.89 to 6.49 N/mm; p = 0.002) and Vicryl rapide (from 2.84 to 10.5 N/mm; p = 0.007) revealed an increasing stiffness over time (see Fig. 4). Maxon and Ethibond had stable stiffness values over the 2-month test period without significant differences between the measurement points. PDS showed constant values until day 42; afterwards, the stiffness increased (from 2.40 to 3.44 N/mm; p = 0.014). Monocryl on the other hand had a decreasing stiffness between day 14 and 28 (from 1.09 to 0.42 N/mm; p < 0.001).
As in the measurements of maximal strain, PDS and Ethibond had constant hysteresis values over the time course (see Fig. 5). The Maxon loop revealed decreasing hysteresis (from 36.3 to 15.9 %; p = 0.004). In contrast, both Vicryl (from 47.6 to 51.2 %; p = 0.053) and Monocryl (from 20.1 to 27.0 %; p < 0.001) had increasing hysteresis with ongoing degradation.
Soft tissue such as the tendons, fascia, ligaments, or skin are often surgically positioned and fixed using surgical suture material. In comparison to other surgical specialties, orthopedic surgery features particularly forces with repetitive loading on the repair site that can jeopardize appropriate healing. While suture retention in the tissue is one major issue, failure of the suture itself is common. Further, the act of seating the stitch and knot may lead to suture loop elongation and gap formation, events that may also lead to compromised healing . These factors should be considered by the surgeon when choosing an appropriate suture material, particularly with regard to load bearing capacity and elasticity of the suture material.
Numerous choices for a suture material are available, including biodegradable sutures. Biodegradable material can be viewed as well suited for applications in which the suture is no longer required after healing has occurred. However, for repairs of tissues that are subjected to high mechanical demands, degradable sutures are often not utilized by the surgeon. This has mainly to do with uncertainty regarding the expected duty life of the sutures related to their progressive hydrolysis and corresponding loss of mechanical integrity. While several studies have described the biomechanical properties of large diameter surgical sutures in various conditions, these studies neglect the effect of time [12, 14, 19, 20].
Therefore, the aim of this study was to provide data on the mechanical properties of the most common suture materials used in orthopedics. In particular, the changes of the material properties during an observation period of 56 days were investigated.
One limitation of this study was the use of an in vitro conditioning of the materials that did not comprise cyclic load. Such loads can be expected to result in material creep, and how this effect may influence the long-term properties of the sutures may be considered in future tests. In any case, there were no significant differences in load to failure with and without cyclic load. The environmental factors during the incubation time (pH 7.4 and temperature 37 ° C) were standardized using an approved standard testing solution to simulate appropriate values as in vivo. Regarding the here investigated mechanical properties, we are confident that using standardized in vitro conditions simulating the wet and warm milieu of the body reproduces the in vivo conditions adequately. Using an in vivo model would be useful to test the combined development of tissue and suture, but would be less useful to test the development of the suture properties alone.
We confirmed that Vicryl rapide and Monocryl lose their mechanical strength relatively quickly, with an effective loss of integrity after an incubation period of 14 and 28 days, respectively. Due to the early degradation, other properties including maximal strain and stiffness also showed significant changes in the first weeks. These materials appear to be only suitable for situations in which rapid healing is expected, with minimal longer-term mechanical demands. This would concern applications such as in ligations or skin closure, where for example subcutaneous irritation makes early absorption desirable.
Regarding the consequences on the best choice of suture material for the orthopedic surgeon, of course the final decision is to be made by individual surgeon. However, in the case of degrading sutures, there is a race between increasing strength of the developing scar and decrease of the sutures properties. Scar healing occurs with a speed of roughly 25 % at 6 weeks, 45 % at 12 weeks, and 80 % at 24 weeks of the final strength . Therefore, the suture should correspondingly preserve 75, 55, and 20 % at the according time points. Particularly, the elasticity of the suture may be beneficial to compensate for sudden but rare spikes in loading on the suture-repair construct, in order to prevent failure or breakage. We could show that particularly PDS will preserve its advantageous properties over the time of absorption, with corresponding lower maximum tensile strength.
The three absorbable sutures Vicryl, PDS, and Maxon all could sustain higher loads during the first 2 weeks than the non-absorbable Ethibond. As expected, the properties of the non-absorbable Ethibond did not differ over time. Unexpectedly, also Maxon and PDS maintained their elastic properties in spite of their proceeding degradation and loss of tensile strength. Thus, even after considerable loss of failure strength, the relative elasticity of these materials remained intact and the suture could still be expected to adequately support transient tissue loads. However, while PDS may be considered useful to bear clinically relevant loads on the tendon, ligaments, or bone, Maxon and Vicryl may be rather considered where mechanically less challenged adaptation of tissue is performed such as in closure of peritendineum, side-to-side repairs of fascia, and similar situations.
In summary, this is the first study assessing the properties of large-diameter degradable sutures during a time period relevant for orthopedic applications. The non-absorbable Ethibond and surprisingly the absorbable Maxon and PDS revealed relatively constant values despite the process of degradation.
The choice of an appropriate suture material should consider the expected duty loads in context of tissue healing time. The data we present provides some guidance to the orthopedic surgeon in better predicting the long-term performance of suture materials used everyday in surgical practice.
United States Pharmacopeia
Baring TK, Cashman PP, Reilly P, Emery RJ, Amis AA. Rotator cuff repair failure in vivo: a radiostereometric measurement study. J Shoulder Elbow Surg. 2011;20(8):1194–9. doi:10.1016/j.jse.2011.04.010.
Gerber C, Schneeberger AG, Perren SM, Nyffeler RW. Experimental rotator cuff repair. A preliminary study. J Bone Joint Surg Am. 1999;81(9):1281–90.
Chu CC, Moncrief G. An in vitro evaluation of the stability of mechanical properties of surgical suture materials in various pH conditions. Annals of surgery. 1983;198(2):223-8.
Freudenberg S, Rewerk S, Kaess M, Weiss C, Dorn-Beinecke A, Post S. Biodegradation of absorbable sutures in body fluids and pH buffers. Eur Surg Res. 2004;36(6):376–85. doi:10.1159/000081648.
Tomihata K, Suzuki M, Ikada Y. The pH dependence of monofilament sutures on hydrolytic degradation. J Biomed Mater Res. 2001;58(5):511–8. doi:10.1002/jbm.1048.
Debus ES, Geiger D, Sailer M, Ederer J, Thiede A. Physical, biological and handling characteristics of surgical suture material: a comparison of four different multifilament absorbable sutures. Eur Surg Res. 1997;29(1):52–61.
Greenwald D, Shumway S, Albear P, Gottlieb L. Mechanical comparison of 10 suture materials before and after in vivo incubation. J Surg Res. 1994;56(4):372–7. doi:10.1006/jsre.1994.1058.
Lunstedt B, Knoop M, Thiede A. Review of the physical and surgical technical properties of modern monofilament suture materials. Chirurg. 1986;57(8):510–3.
Metz SA, Chegini N, Masterson BJ. In vivo and in vitro degradation of monofilament absorbable sutures, PDS and Maxon. Biomaterials. 1990;11(1):41–5.
Sugimachi K, Sufian S, Weiss MJ, Pavlides CA, Matsumoto T. Evaluation of absorbable suture materials in biliary tract surgery. Int Surg. 1978;63(3):135–9.
Barber FA, Herbert MA, Richards DP. Sutures and suture anchors: update 2003. Arthroscopy. 2003;19(9):985–90.
Barber FA, Herbert MA, Beavis RC. Cyclic load and failure behavior of arthroscopic knots and high strength sutures. Arthroscopy. 2009;25(2):192–9. doi:10.1016/j.arthro.2008.09.010.
Barber FA, Herbert MA, Coons DA, Boothby MH. Sutures and suture anchors—update 2006. Arthroscopy. 2006;22(10):1063–e1061-1069. doi:10.1016/j.arthro.2006.04.106.
Najibi S, Banglmeier R, Matta J, Tannast M. Material properties of common suture materials in orthopaedic surgery. Iowa Orthop J. 2010;30:84–8.
Swan Jr KG, Baldini T, McCarty EC. Arthroscopic suture material and knot type: an updated biomechanical analysis. Am J Sports Med. 2009;37(8):1578–85. doi:10.1177/0363546509332816.
Wright PB, Budoff JE, Yeh ML, Kelm ZS, Luo ZP. The properties of damaged and undamaged suture used in metal and bioabsorbable anchors: an in vitro study. Arthroscopy. 2007;23(6):655–61. doi:10.1016/j.arthro.2007.01.008.
1635-04 AF (ed) (2004) A standard test method for in vitro degeneration testing of hydrolytically degradable polymer resins and fabricated forms for surgical implants. Annual Book of ASTM Standards, Philadelphia.
Dinopoulos HT, Boyer MI, Burns ME, Gelberman RH, Silva MJ. The resistance of a four- and eight-strand suture technique to gap formation during tensile testing: an experimental study of repaired canine flexor tendons after 10 days of in vivo healing. J Hand Surg Am. 2000;25(3):489–98. doi:10.1053/jhsu.2000.6456.
Ilahi OA, Younas SA, Ho DM, Noble PC. Security of knots tied with ethibond, fiberwire, orthocord, or ultrabraid. Am J Sports Med. 2008;36(12):2407–14. doi:10.1177/0363546508323745.
Wright PB, Budoff JE, Yeh ML, Kelm ZS, Luo ZP. Strength of damaged suture: an in vitro study. Arthroscopy. 2006;22(12):1270–5. doi:10.1016/j.arthro.2006.08.019. e1273.
We thank the Orthopedic Department of the Balgrist University Hospital to provide the suture materials and the needed infrastructure for incubation and measurements.
The Orthopedic Department of the Balgrist University Hospital provided the suture materials and the infrastructure for incubation and measurements. There was no other source of funding.
Availability of data and materials
The results of the measurements are saved online using “organized lab” from LabArchives, LLC (Carlsbad, CA 92008, USA). The dataset supporting the conclusions of this article is available in the Experimental Data/Absorbable Fiber repository, doi:10.6070/H4HH6H4J. The data is accessible via hyperlink: https://mynotebook.labarchives.com/share/Daniel%2520M%25C3%25BCller/MjAuOHw5MTM3MS8xNi9UcmVlTm9kZS8zNDg2MzQ5NDU5fDUyLjg.
DAM carried out all the preparations and the measurements of the study and drafted the manuscript. JGS participated in the design of the study and supervised the analysis of the mechanical properties and the statistical analysis. DCM conceived of the study and participated in its design and coordination and helped to draft the manuscript. All authors read and approved the final manuscript.
The authors declare that they have no competing interests.
Consent for publication
Ethics approval and consent to participate
Rights and permissions
Open Access This article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The Creative Commons Public Domain Dedication waiver (http://creativecommons.org/publicdomain/zero/1.0/) applies to the data made available in this article, unless otherwise stated.
About this article
Cite this article
Müller, D.A., Snedeker, J.G. & Meyer, D.C. Two-month longitudinal study of mechanical properties of absorbable sutures used in orthopedic surgery. J Orthop Surg Res 11, 111 (2016). https://doi.org/10.1186/s13018-016-0451-5
- Absorbable fiber
- Material properties
- In vitro
- Orthopedic surgery